TENSILE TESTS (ASTM D 638, ISO


 Jeremy McKenzie
 9 months ago
 Views:
Transcription
1 MODULE 4 The mechanical properties, among all the properties of plastic materials, are often the most important properties because virtually all service conditions and the majority of enduse applications involve some degree of mechanical loading. Nevertheless, these properties are the least understood by most design engineers. The material selection for a variety of applications is quite often based on mechanical properties such as tensile strength, modulus, elongation, and impact strength. The basic understanding of stress strain behavior of plastic materials is of utmost importance to design engineers. One such typical stress strain (loaddeformation) diagram is illustrated in Figure 21. For a better understanding of the stress strain curve, it is necessary to define a few basic terms that are associated with the stress strain diagram. Stress. The force applied to produce deformation in a unit area of a test specimen. Stress is a ratio of applied load to the original crosssectional area expressed in lb/in.2. Strain. The ratio of the elongation to the gauge length of the test specimen, or simply stated, change in length per unit of the original length ( l/l). t is expressed as a dimensionless ratio. Elongation. The increase in the length of a test specimen produced by a tensile load. Yield Point. The fi rst point on the stress strain curve at which an increase in strain occurs without the increase in stress. Yield Strength. The stress at which a material exhibits a specifi ed limiting deviation from the proportionality of stress to strain. Unless otherwise specified, this stress will be at the yield point. Proportional Limit. The greatest stress at which a material is capable of sustaining the applied load without any deviation from proportionality of stress to strain (Hooke s Law). This is expressed in lb/in.2.
2 Modulus of Elasticity. The ratio of stress to corresponding strain below the proportional limit of a material. t is expressed in F/A, usually lb/in.2 This is also known as Young s modulus. A modulus is a measure of material s stiffness. Ultimate Strength. The maximum unit stress a material will withstand when subjected to an applied load in compression, tension, or shear. This is expressed in lb/in.2. Secant Modulus. The ratio of the total stress to corresponding strain at any specific point on the stress strain curve. t is also expressed in F/A or lb/in.2. The stress strain diagram illustrated in Figure 21 is typical of that obtained in tension for a constant rate of loading. However, the curves obtained from other loading conditions, such as compression or shear, are quite similar in appearance. The initial portion of the stress strain curve between points A and C is linear and it follows Hooke s law, which states that for an elastic material the stress is proportional to the strain. The point C at which the actual curve deviates from the straight line is called the proportional limit, meaning that only up to this point is stress proportional to strain. The behavior of plastic material below the proportional limit is elastic in nature and therefore the deformations are recoverable. The deformations up to point B in Figure 21 are relatively small and have been associated with the bending and stretching of the interatomic bonds between atoms of plastic molecules as shown in Figure 22a. This type of deformation is instantaneous and recoverable. There is no permanent displacement of the molecules relative to each other. The deformation that occurs beyond point C in Figure 21 is similar to a straightening out of a coiled portion of the molecular chains (Figure22b). There is no intermolecular slippage and the deformations may be recoverable ultimately, but not instantaneously. The extensions that occur beyond the yield point or the elastic limit of the material are not recoverable (Figure 22c). There deformations occur because of the actual displacement of the molecules with respect to each other. The displaced molecules cannot slip back to their original positions and, therefore, a permanent deformation or set occurs. These three types of deformations, as shown in Figure 22, do not occur separately but are superimposed on each other. The bonding and the stretching of the interatomic bonds are almost instantaneous. However, the molecular uncoiling is relatively slow. Molecular slippage effects are the slowest of all three deformations The polymeric materials can be broadly classifi ed in terms of their relative softness, brittleness, hardness, and toughness. The tensile stress strain diagrams serve as a basis for such a classifi cation (6). The area under the stress strain
3 curve is considered as the toughness of the polymeric material. Figure 24a illustrates typical tensile stress strain curves for several types of polymeric materials. A soft and weak material is characterized by low modulus, low yield stress, and a moderate elongation at break point. Polytetrafl uoroethylene (PTFE) is a good example of one such type of plastic material. A soft but tough material shows low modulus and low yield stress, but very high elongation and high stress at break. Polyethylene is a classic example of these types of plastics. A hard and brittle material is characterized by high modulus and low elongation. t may or may not yield before breaking. One such type of polymer is general purpose phenolic. A hard and strong material has high modulus, high yield stress, usually high ultimate strength, and low elongation. Acetal is a good example of this class of materials. A hard and tough material is characterized by high modulus, high yield stress, high elongation at break, and high ultimate strength. Polycarbonate is considered a hard and tough material. Figure 24b illustrates the relation between ductility and strength. TENSLE TESTS (ASTM D 638, SO 5271) Tensile elongation and tensile modulus measurements are among the most important indications of strength in a material and are the most widely specified properties of plastic materials. Tensile test, in a broad sense, is a measurement of the ability of a material to withstand forces that tend to pull it apart and to determine to what extent the material stretches before breaking. Tensile modulus, an indication of the relative stiffness of a material, can be determined from a stress strain diagram. Different types of plastic materials are often compared on the basis of tensile strength, elongation, and tensile modulus data. Many plastics are very sensitive to the rate of straining and environmental conditions. Apparatus The tensile testing machine of a constantrateofcrosshead movement is used. t has a fi xed or essentially stationary member carrying one grip, and a movable member carrying a second grip. Selfaligning grips employed for holding the test specimen between the fixed member and the movable member prevent alignment problems. A controlledvelocity drive mechanism is used. Some of the commercially available machines use a closedloop servocontrolled drive mechanism to provide a high degree of speed accuracy. Test Specimens and Conditioning Test specimens for tensile tests are prepared many different ways. Most often, they are either injection molded or compression molded. The specimens may also be prepared by machining operations from materials in sheet, plate, slab, or similar form. Test specimen dimensions vary considerably depending upon the requirements and are
4 described in detail in the ASTM book of standards. Figure 29 shows ASTM D 638 Type tensile test specimen most commonly used for testing rigid and semirigid plastics. The specimens are conditioned using standard conditioning procedures. Since the tensile properties of some plastics change rapidly with small changes in temperature, it is recommended that tests be conducted in the standard laboratory atmosphere of 23 } 2 C and 50 } 5 percent relative humidity. Test Procedures A. Tensile Strength The speed of testing is the relative rate of motion of the grips or test fixtures during the test. There are basically five different testing speeds specified in the ASTM D638 Standard. The most frequently employed speed of testing is 0.2 in./min. Whenever possible, the speed indicated by the specification for the material being tested should be used. f a test speed is not given, appropriate speed that causes rupture between 30 sec and 5 min should be chosen. The test specimen is positioned vertically in the grips of the testing machine. The grips are tightened evenly and firmly to prevent any slippage. The speed of testing is set at the proper rate and the machine is started. As the specimen elongates, the resistance of the specimen increases and is detected by a load cell. This load value (force) is recorded by the instrument. Some machines also record the maximum (peak) load obtained by the specimen, which can be recalled after the completion of the test. The elongation of the specimen is continued until a rupture of the specimen is observed. Load value at break is also recorded. The tensile strength at yield and at break (ultimate tensile strength) are calculated. B. Tensile Modulus and Elongation Tensile modulus and elongation values are derived from a stress strain curve. An extensometer is attached to the test specimen as shown in Figure 210a. The extensometer is a strain gauge type of device that magnifi es the actual stretch of the specimen considerably. Reliability of the strain measurement is affected by the traditional contact extensometers due to the actual physical contact with the test specimen. n recent years, many test equipment manufacturers have developed noncontact measurement systems based on optical, video and laser devices to overcome problems associated with contact extensometers. FLEXURAL PROPERTES (ASTM D 790, SO 178) The stress strain behavior of polymers in fl exure is of interest to a designer as well as a polymer manufacturer. Flexural strength is the ability of the material to withstand bending forces applied perpendicular to its longitudinal axis. The stresses induced by the fl exural load are a combination of compressive and tensile stresses. This effect is illustrated in Figure Flexural properties are reported are reported and calculated in terms of the maximum stress and strain that occur at the outside surface of the test bar. Many polymers do not break under fl exure even after a large defl ection that makes determination of the ultimate fl exural strength impractical for many polymers. n such cases, the common practice is to report fl exural yield strength when the maximum strain in the outer fi ber of the specimen has reached 5 percent. For polymeric materials that break easily under fl exural load, the specimen is defl ected until a rupture occurs in the outer fi bers. Figure Forces involved in bending a simple beam.
5 There are several advantages of fl exural strength tests over tensile tests (14). f a material is used in the form of a beam and if the service failure occurs in bending, then a fl exural test is more relevant for design or specifi cation purposes than a tensile test, which may give a strength value very different from the calculated strength of the outer fi ber in the bent beam. The fl exural specimen is comparatively easy to prepare without residual strain. The specimen alignment is also more difficult in tensile tests. Also, the tight clamping of the test specimens creates stress concentration points. One other advantage of the fl exural test is that at small strains, the actual deformations are suffi ciently large to be measured accurately. There are two basic methods that cover the determination of flexural properties of plastics. Method 1 is a threepoint loading system utilizing center loading on a simple supported beam. A bar of rectangular cross section rests on two supports and is loaded by means of a loading nose midway between the supports. The maximum axial fiber stresses occur on a line under the loading nose. A closeup of a specimen in the testing apparatus is shown in Figure This method is especially useful in determining flexural properties for quality control and specification purposes. Method 2 is a fourpoint loading system utilizing two load points equally spaced from their adjacent support points, with a distance between load points of onethird of the support span. n this method, the test bar rests on two supports and is loaded at two points (by means of two loading noses), each an equal distance from the adjacent support point. This arrangement is shown schematically in Figure Method 2 is very useful in testing material that do not fail at the point of maximum stress under a threepoint loading system. The maximum axial fiber stress occurs over the area between the loading noses. Apparatus Quite often, the machine used for tensile testing is also used for flexural testing. The upper or lower portion of the movable crosshead can be used for flexural testing. The loading nose and support must have cylindrical surfaces. The radius of the nose and the nose support should be at least 1/8 in. to avoid excessive indentation or failure due to stress concentration directly under the loading nose. A strain gauge type of mechanism called a deflectometer or compressometer is used to measure defl ection in the specimen. Test Specimens and Conditioning The specimens used for fl exural testing are bars of rectangular cross section and are cut from sheets, plates, or molded shapes. The common practice is to mold the specimens to the desired fi nished dimensions. The specimens are conditioned in accordance with Procedure A of ASTM methods D618 as explained in Chapter 11 of this book. The specimens of size 1/8 1/2 4 in. are the most commonly used. Test Procedures and Calculations The test is initiated by applying the load to the specimen at the specifi ed crosshead rate. The defl ection is measured either by a gauge under the specimen in contact with it in the center of the support span or by measurement of the motion of the loading nose relative to the supports. A load defl ection curve is plotted if the determination of fl exural modulus value is desired. The maximum fi ber stress is related to the load and sample dimensions and is calculated using the following equation: where S = stress (psi); P = load (lb); L = length of span (in.); b = width of specimen (in.); d = thickness of specimen (in.). Flexural strength is equal to the maximum stress in the outer fibers at the moment of break. This value can be calculated by using the above stress equation by letting load value P equal the load at the moment of break. For materials that do not break at outer fiber strains up to 5 percent, the flexural yield strength is calculated using the same equation. The load value P in this case is the maximum load at which there is no longer an increase in load with an increase in deflection. Modulus of Elasticity (Flexural Modulus) The fl exural modulus is a measure of the stiffness during the fi rst or initial part of the bending process. The fl exural modulus is represented by the slope of the initial straightline portion of the stress strain curve and is calculated by dividing the change in stress by the corresponding change in strain. The procedure to calculate flexural modulus is similar to the one described previously for tensile modulus calculations.
6 Mechanical Behaviour of Plastics 85 they do aid in the understanding and analysis of the behaviour of viscoelastic materials. Some of the more important models will now be considered. (a) Maxwell Model The Maxwell Model consists of a spring and dashpot in series at shown in Fig This model may be analysed as follows. Fig The Maxwell model StressStrain Relations The spring is the elastic component of the response and obeys the relation O'1  ~'E1 (2.27) where Crl and el are the stress and strain respectively and ~ is a constant. The dashpot is the viscous component of the response and in this case the stress t~2 is proportional to the rate of strain e2, ie where r/is a material constant. Equilibrium Equation For equilibrium of forces, assuming constant area Geometry of Deformation Equation ~2 = ~" k2 (2.28) Applied Stress, cr ttl = ~2 (2.29) The total strain, e is equal to the sum of the strains in the two elements. So ~ ~l ~" ~2 (2.30)
7 86 Mechanical Behaviour of Plastics From equations (2.27), (2.28) and (2.30) 1 1 k = 'Sbl +0"2 r/ 1 1 k b o (2.31) o This is the governing equation of the Maxwell Model. t is interesting to consider the response that this model predicts under three common timedependent modes of deformation. (i) Creep f a constant stress, cro, is applied then equation (2.31) becomes 1 = .tro (2.32) r/ which indicates a constant rate of increase of strain with time. From Fig it may be seen that for the Maxwell model, the strain at any time, t, after the application of a constant stress, tro, is given by Cro e ( t ) = ( + tr~ bt d 41 q/) llb _(To r 0 tl L L"% Relaxation 1 1 tl! t _ J i 6'='~" Recovery Z t2  Time Time Fig Response of Maxwell model
8 Mechanical Behaviour of Plastics 87 Hence, the creep modulus, E(t), is given by (ii) Relaxation E(t) = = (2.33) e(t) r/4/~t f the strain is held constant then equation (2.31) becomes 1 1 0= &+.or Solving this differential equation (see Appendix B) with the initial condition e = Cro at t = to then, ~t cr(t) = croe n (2.34) tr(t) =tro et/tr (2.35) where TR = r//~ is referred to as the relaxation time. This indicates that the stress decays exponentially with a time constant of r//~ (see Fig. 2.35). (iii) Recovery When the stress is removed there is an instantaneous recovery of the elastic strain, e, and then, as shown by equation (2.31), the strain rate is zero so that there is no further recovery (see Fig. 2.35). t can be seen therefore that although the relaxation behaviour of this model is acceptable as a first approximation to the actual materials response, it is inadequate in its prediction for creep and recovery behaviour. (b) Kelvin or Voigt Model n this model the spring and dashpot elements are connected in parallel as shown in Fig Fig The Kelvin or Voigt Model
9 88 Mechanical Behaviour of Plastics StressStrain Relations These are the same as the Maxwell Model and are given by equations (2.27) and (2.28). Equilibrium Equation For equilibrium of forces it can be seen that the applied load is supported jointly by the spring and the dashpot, so Geometry of Deformation Equation cr = crl + or2 (2.36) n this case the total strain is equal to the strain in each of the elements, i.e. From equations (2.27), (2.28) and (2.36) e = el = e2 (2.37) cr = ~. el + Ok2 or using equation (2.37) tr = ~. e + r/. k (2.38) This is the governing equation for the Kelvin (or Voigt) Model and it is interesting to consider its predictions for the common time dependent deformations. (i) Creep f a constant stress, %, is applied then equation (2.38) becomes ao=~.e+o~ and this differential equation may be solved for the total strain, e, to give e(t) = ~ le where the ratio r//~ is referred to as the retardation time, TR. This indicates an exponential increase in strain from zero up to the value, tro/~, that the spring would have reached if the dashpot had not been present. This is shown in Fig As for the Maxwell Model, the creep modulus may be determined as oo [,], E(t) = 6(0 = ~" 1  e~ (2.39)
10 Mechanical Behaviour of Plastics 89 t Asymptote ~ = ao/p,... ~T... %1 _t"",~' i "=Creep.~" i L\ Recow, y ~ h '<i i 0 tl t2 Time Relaxation  ao 0 i! i,, 0 tl t 2 v Time Fig Response of Kelvin/Voigt model (ii) Relaxation f the strain is held constant then equation (2.38) becomes That is, the stress is constant and supported by the spring element so that the predicted response is that of an elastic material, i.e. no relaxation (see Fig. 2.37) (iii) Recovery f the stress is removed, then equation (2.38) becomes 0=~.e+o~ Solving this differential equation with the initial condition e = e' at the time of stress removal, then e(t) = e'e ~ (2.40) This represents an exponential recovery of strain which is a reversal of the predicted creep. (c) More Complex Models t may be seen that the simple Kelvin model gives an acceptable first approximation to creep and recovery behaviour but does not account for relaxation. The Maxwell model can account for relaxation but was poor in relation to creep
11 90 Mechanical Behaviour of Plastics and recovery. t is clear therefore that some compromise may be achieved by combining the two models. Such a setup is shown in Fig n this case the stressstrain relations are again given by equations (2.27) and (2.28). The geometry of deformation yields. Total strain, e = e~ + e2  ek (2.41) Fig Maxwell and Kelvin models in series where ek is the strain response of the Kelvin Model. From equations (2.27), (2.28) and (2.41). tro trot Cro[ _~gz!] g ( t ) = ~l "~" g] " + ~ e ~2 (2.42) From this the strain rate may be obtained as ~ = r b cro ~t ~ ~e,~2 (2.43) r/1 r/2 The response of this model to creep, relaxation and recovery situations is the sum of the effects described for the previous two models and is illustrated in Fig t can be seen that although the exponential responses predicted in these models are not a true representation of the complex viscoelastic response of polymeric materials, the overall picture is, for many purposes, an acceptable approximation to the actual behaviour. As more and more elements are added to the model then the simulation becomes better but the mathematics become complex. Example 2.12 An acrylic moulding material is to have its creep behaviour simulated by a four element model of the type shown in Fig f the creep curve for the acrylic at 14 MN/m 2 is as shown in Fig. 2,40, determine the values of the four constants in the model.
12 Mechanical Behaviour of Plastics 91 J Recovery ~_ ao! o i.... tl... t2 nm~ e = ~ 2 0 Oo ~,' i... l i t~ t2.... F Time Fig Response of combined Maxwell and Kelvin models Stres~ MNm 2 C " ~ ~ / , Slope = ~ = X 10 "s hr 1 o ~oo 2oo ~o ~ Time (hours) Fig Creep curve for acrylic at 20~ Solution The spring element constant, ~1, for the Maxwell model may be obtained from the instantaneous strain, e~. Thus ~1 = O'~ = MN/m 2 el The dashpot constant, 01, for the Maxwell element is obtained from the slope of the creep curve in the steady state region (see equation (2.32)). tro 14 r/1 = ~ = = 1.2 x 107 MN.hr/m 2 e x 106 = 4.32 x 10 l~ MN.s/m 2
13 92 Mechanical Behaviour of Plastics The spring constant, ~2, for the KelvinVoigt element is obtained from the maximum retarded strain, e2, in Fig ~ o = 14 = 7000 MN/m 2 e2 ( )102 The dashpot constant, 0z, for the KelvinVoigt element may be determined by selecting a time and corresponding strain from the creep curve in a region where the retarded elasticity dominates (i.e. the knee of the curve in Fig. 2.40) and substituting into equation (2.42). f this is done then 02 = 3.7 x 108 MN.s/m 2. Having thus determined the constants for the model the strain may be predicted for any selected time or stress level assuming of course these are within the region where the model is applicable. (d) Standard Linear Solid Another model consisting of elements in series and parallel is that attributed to Zener. t is known as the Standard Linear Solid and is illustrated in Fig The governing equation may be derived as follows. Fig The standard linear solid StressStrain Relations As shown earlier the stressstrain relations are 0.1 ~ ~E1 0" 2 =~2E2 0"3 " ~3~3 (2.44) (2.45) (2.46) Equilibrium Equation n a similar manner to the previous models, equilibrium of forces yields. 0.1 "0"3 tr = trl + a2 (2.47)
Mechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationPhysical Properties Testing Technical Bulletin
Technical Bulletin MANUFACTURER Raven Lining Systems 13105 E. 61 st Street, Suite A Broken Arrow, OK 74012 (918) 6150020 TENSILE TESTING OF PLASTICS ASTM D638, ISO 527 Tensile tests measure the force
More informationSTANDARD SAMPLE. Reduced section " Diameter. Diameter. 2" Gauge length. Radius
MATERIAL PROPERTIES TENSILE MEASUREMENT F l l 0 A 0 F STANDARD SAMPLE Reduced section 2 " 1 4 0.505" Diameter 3 4 " Diameter 2" Gauge length 3 8 " Radius TYPICAL APPARATUS Load cell Extensometer Specimen
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationME 243. Mechanics of Solids
ME 243 Mechanics of Solids Lecture 2: Stress and Strain Ahmad Shahedi Shakil Lecturer, Dept. of Mechanical Engg, BUET Email: sshakil@me.buet.ac.bd, shakil6791@gmail.com Website: teacher.buet.ac.bd/sshakil
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationME 2570 MECHANICS OF MATERIALS
ME 2570 MECHANICS OF MATERIALS Chapter III. Mechanical Properties of Materials 1 Tension and Compression Test The strength of a material depends on its ability to sustain a load without undue deformation
More informationModule4. Mechanical Properties of Metals
Module4 Mechanical Properties of Metals Contents ) Elastic deformation and Plastic deformation ) Interpretation of tensile stressstrain curves 3) Yielding under multiaxial stress, Yield criteria, Macroscopic
More informationTensile stress strain curves for different materials. Shows in figure below
Tensile stress strain curves for different materials. Shows in figure below Furthermore, the modulus of elasticity of several materials effected by increasing temperature, as is shown in Figure Asst. Lecturer
More informationThe science of elasticity
The science of elasticity In 1676 Hooke realized that 1.Every kind of solid changes shape when a mechanical force acts on it. 2.It is this change of shape which enables the solid to supply the reaction
More informationLab Exercise #5: Tension and Bending with Strain Gages
Lab Exercise #5: Tension and Bending with Strain Gages Prelab assignment: Yes No Goals: 1. To evaluate tension and bending stress models and Hooke s Law. a. σ = Mc/I and σ = P/A 2. To determine material
More informationHigh Tech High Top Hat Technicians. An Introduction to Solid Mechanics. Is that supposed to bend there?
High Tech High Top Hat Technicians An Introduction to Solid Mechanics Or Is that supposed to bend there? Why don't we fall through the floor? The power of any Spring is in the same proportion with the
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationAERO 214. Lab II. Measurement of elastic moduli using bending of beams and torsion of bars
AERO 214 Lab II. Measurement of elastic moduli using bending of beams and torsion of bars BENDING EXPERIMENT Introduction Flexural properties of materials are of interest to engineers in many different
More informationMATERIALS. Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle?
MATERIALS Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: A. Composition
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationCreep. Creep behavior of viscoelastic polymeric materials
B1 Version: 2.2_EN Date: 15. March 2018. BUDAPEST UNIVERSITY OF TECHNOLOGY AND ECONOMICS FACULTY OF MECHANICAL ENGINEERING DEPARTMENT OF POLYMER ENGINEERING Creep Creep behavior of viscoelastic polymeric
More informationJohns Hopkins University What is Engineering? M. Karweit MATERIALS
Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: MATERIALS A. Composition
More informationFlexural properties of polymers
A2 _EN BUDAPEST UNIVERSITY OF TECHNOLOGY AND ECONOMICS FACULTY OF MECHANICAL ENGINEERING DEPARTMENT OF POLYMER ENGINEERING Flexural properties of polymers BENDING TEST OF CHECK THE VALIDITY OF NOTE ON
More informationStress Strain Elasticity Modulus Young s Modulus Shear Modulus Bulk Modulus. Case study
Stress Strain Elasticity Modulus Young s Modulus Shear Modulus Bulk Modulus Case study 2 In field of Physics, it explains how an object deforms under an applied force Real rigid bodies are elastic we can
More informationGEOSYNTHETICS ENGINEERING: IN THEORY AND PRACTICE
GEOSYNTHETICS ENGINEERING: IN THEORY AND PRACTICE Prof. J. N. Mandal Department of Civil Engineering, IIT Bombay, Powai, Mumbai 400076, India. Tel.02225767328 email: cejnm@civil.iitb.ac.in Module13 LECTURE
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More informationThe objective of this experiment is to investigate the behavior of steel specimen under a tensile test and to determine it's properties.
Objective: The objective of this experiment is to investigate the behavior of steel specimen under a tensile test and to determine it's properties. Introduction: Mechanical testing plays an important role
More information22 Which of the following correctly defines the terms stress, strain and Young modulus? stress strain Young modulus
PhysicsndMathsTutor.com Which of the following correctly defines the terms stress, strain and Young modulus? 97/1/M/J/ stress strain Young modulus () x (area) (extension) x (original length) (stress) /
More informationPOE Practice Test  Materials
Class: Date: POE Practice Test  Materials Multiple Choice Identify the choice that best completes the statement or answers the question. 1. A student weighs 150 lbs and is standing on a beam which spans
More informationTINIUS OLSEN Testing Machine Co., Inc.
Interpretation of StressStrain Curves and Mechanical Properties of Materials Tinius Olsen has prepared this general introduction to the interpretation of stressstrain curves for the benefit of those
More informationQUESTION BANK DEPARTMENT: CIVIL SEMESTER: III SUBJECT CODE: CE2201 SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A
DEPARTMENT: CIVIL SUBJECT CODE: CE2201 QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State
More informationHow materials work. Compression Tension Bending Torsion
Materials How materials work Compression Tension Bending Torsion Elemental material atoms: A. Composition a) Nucleus: protons (+), neutrons (0) b) Electrons () B. Neutral charge, i.e., # electrons = #
More informationLecture 8 Viscoelasticity and Deformation
Read: pg 130 168 (rest of Chpt. 4) 1 Poisson s Ratio, µ (pg. 115) Ratio of the strain in the direction perpendicular to the applied force to the strain in the direction of the applied force. For uniaxial
More informationINTRODUCTION TO STRAIN
SIMPLE STRAIN INTRODUCTION TO STRAIN In general terms, Strain is a geometric quantity that measures the deformation of a body. There are two types of strain: normal strain: characterizes dimensional changes,
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More information12/8/2009. Prof. A.K.M.B. Rashid Department of MME BUET, Dhaka
Prof. A.K.M.B. Rashid Department of MME BUET, Dhaka Introduction and classes of properties Case studies showing selection of the right material for the job Deformation of material under the action of a
More informationBioMechanics and BioMaterials Lab (BME 541) Experiment #5 Mechanical Prosperities of Biomaterials Tensile Test
BioMechanics and BioMaterials Lab (BME 541) Experiment #5 Mechanical Prosperities of Biomaterials Tensile Test Objectives 1. To be familiar with the material testing machine(810le4) and provide a practical
More informationFIS Specifications for Flex Poles (Edition May 2008) Original Text: German
FIS Specifications for Flex Poles (Edition May 2008) Original Text: German 1 Field of Application and Basic Information The following FIS specifications for flex poles are intended to ensure that flex
More informationQUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS
QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State Hooke s law. 3. Define modular ratio,
More informationDEPARTMENT OF MECHANICAL ENIGINEERING, UNIVERSITY OF ENGINEERING & TECHNOLOGY LAHORE (KSK CAMPUS).
DEPARTMENT OF MECHANICAL ENIGINEERING, UNIVERSITY OF ENGINEERING & TECHNOLOGY LAHORE (KSK CAMPUS). Lab Director: Coordinating Staff: Mr. Muhammad Farooq (Lecturer) Mr. Liaquat Qureshi (Lab Supervisor)
More informationPERIYAR CENTENARY POLYTECHNIC COLLEGE PERIYAR NAGAR  VALLAM THANJAVUR. DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK
PERIYAR CENTENARY POLYTECHNIC COLLEGE PERIYAR NAGAR  VALLAM  613 403  THANJAVUR. DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK Sub : Strength of Materials Year / Sem: II / III Sub Code : MEB 310
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More informationStatics Principles. The laws of motion describe the interaction of forces acting on a body. Newton s First Law of Motion (law of inertia):
Unit 2 Review Statics Statics Principles The laws of motion describe the interaction of forces acting on a body Newton s First Law of Motion (law of inertia): An object in a state of rest or uniform motion
More informationStandard Test Methods for Flexural Properties of Unreinforced and Reinforced Plastics and Electrical Insulating Materials 1
NOTICE: This standard has either been superseded and replaced by a new version or discontinued. Contact ASTM International (www.astm.org) for the latest information. Designation: D 790 00 An American National
More informationMechanical Properties of Materials
Mechanical Properties of Materials Strains Material Model Stresses Learning objectives Understand the qualitative and quantitative description of mechanical properties of materials. Learn the logic of
More informationSTRENGTH OF MATERIALSI. Unit1. Simple stresses and strains
STRENGTH OF MATERIALSI Unit1 Simple stresses and strains 1. What is the Principle of surveying 2. Define Magnetic, True & Arbitrary Meridians. 3. Mention different types of chains 4. Differentiate between
More informationMechanics of Materials Primer
Mechanics of Materials rimer Notation: A = area (net = with holes, bearing = in contact, etc...) b = total width of material at a horizontal section d = diameter of a hole D = symbol for diameter E = modulus
More informationENG1001 Engineering Design 1
ENG1001 Engineering Design 1 Structure & Loads Determine forces that act on structures causing it to deform, bend, and stretch Forces push/pull on objects Structures are loaded by: > Dead loads permanent
More informationBending Load & Calibration Module
Bending Load & Calibration Module Objectives After completing this module, students shall be able to: 1) Conduct laboratory work to validate beam bending stress equations. 2) Develop an understanding of
More information2012 MECHANICS OF SOLIDS
R10 SET  1 II B.Tech II Semester, Regular Examinations, April 2012 MECHANICS OF SOLIDS (Com. to ME, AME, MM) Time: 3 hours Max. Marks: 75 Answer any FIVE Questions All Questions carry Equal Marks ~~~~~~~~~~~~~~~~~~~~~~
More information[5] Stress and Strain
[5] Stress and Strain Page 1 of 34 [5] Stress and Strain [5.1] Internal Stress of Solids [5.2] Design of Simple Connections (will not be covered in class) [5.3] Deformation and Strain [5.4] Hooke s Law
More informationKINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK. Subject code/name: ME2254/STRENGTH OF MATERIALS Year/Sem:II / IV
KINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK Subject code/name: ME2254/STRENGTH OF MATERIALS Year/Sem:II / IV UNIT I STRESS, STRAIN DEFORMATION OF SOLIDS PART A (2 MARKS)
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationCOURSE TITLE : APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4017 COURSE CATEGORY : A PERIODS/WEEK : 6 PERIODS/ SEMESTER : 108 CREDITS : 5
COURSE TITLE : APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4017 COURSE CATEGORY : A PERIODS/WEEK : 6 PERIODS/ SEMESTER : 108 CREDITS : 5 TIME SCHEDULE MODULE TOPICS PERIODS 1 Simple stresses
More informationME 207 Material Science I
ME 207 Material Science I Chapter 3 Properties in Tension and Compression Dr. İbrahim H. Yılmaz http://web.adanabtu.edu.tr/iyilmaz Automotive Engineering Adana Science and Technology University Introduction
More informationA concrete cylinder having a a diameter of of in. mm and elasticity. Stress and Strain: Stress and Strain: 0.
2011 earson Education, Inc., Upper Saddle River, NJ. ll rights reserved. This material is protected under all copyright laws as they currently 8 1. 3 1. concrete cylinder having a a diameter of of 6.00
More informationSTRAIN ANALYSIS OF HDPE BUTT FUSION JOINT IN SIDE BEND TEST
STRAIN ANALYSIS OF HDPE BUTT FUSION JOINT IN SIDE BEND TEST Meng Xiangli (Shawn), McElroy Manufacturing, Inc., Tulsa, OK Abstract The standard practice ASTM F318316 (F3183) has been developed for conducting
More informationMECHANICS OF MATERIALS
Third CHTR Stress MCHNICS OF MTRIS Ferdinand. Beer. Russell Johnston, Jr. John T. DeWolf ecture Notes: J. Walt Oler Texas Tech University and Strain xial oading Contents Stress & Strain: xial oading Normal
More information1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine Spring 2004 LABORATORY ASSIGNMENT NUMBER 6
1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine MIT Spring 2004 LABORATORY ASSIGNMENT NUMBER 6 COMPRESSION TESTING AND ANISOTROPY OF WOOD Purpose: Reading: During this laboratory
More informationME Final Exam. PROBLEM NO. 4 Part A (2 points max.) M (x) y. z (neutral axis) beam crosssec+on. 20 kip ft. 0.2 ft. 10 ft. 0.1 ft.
ME 323  Final Exam Name December 15, 2015 Instructor (circle) PROEM NO. 4 Part A (2 points max.) Krousgrill 11:30AM12:20PM Ghosh 2:303:20PM Gonzalez 12:301:20PM Zhao 4:305:20PM M (x) y 20 kip ft 0.2
More informationPurpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on Exam 3.
ES230 STRENGTH OF MTERILS Exam 3 Study Guide Exam 3: Wednesday, March 8 th inclass Updated 3/3/17 Purpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on
More informationMembers Subjected to Torsional Loads
Members Subjected to Torsional Loads Torsion of circular shafts Definition of Torsion: Consider a shaft rigidly clamped at one end and twisted at the other end by a torque T = F.d applied in a plane perpendicular
More informationChapter Two: Mechanical Properties of materials
Chapter Two: Mechanical Properties of materials Time : 16 Hours An important consideration in the choice of a material is the way it behave when subjected to force. The mechanical properties of a material
More informationProject PAJ2 Dynamic Performance of Adhesively Bonded Joints. Report No. 3 August Proposed Draft for the Revision of ISO
NPL Report CMMT(A)81 Project PAJ2 Dynamic Performance of Adhesively Bonded Joints Report No. 3 August 1997 Proposed Draft for the Revision of ISO 110032 Adhesives  Determination of Shear Behaviour of
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More information9 MECHANICAL PROPERTIES OF SOLIDS
9 MECHANICAL PROPERTIES OF SOLIDS Deforming force Deforming force is the force which changes the shape or size of a body. Restoring force Restoring force is the internal force developed inside the body
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationFlexure: Behavior and Nominal Strength of Beam Sections
4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kipin.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015
More informationMECHANICAL PROPERTIES OF SOLIDS
INTRODUCTION A rigid body generally means a hard solid object having a definite shape and size. But in reality, bodies can be stretched, compressed and bent. Even the appreciably rigid steel bar can be
More informationElastic Properties of Solids (One or two weights)
Elastic properties of solids Page 1 of 8 Elastic Properties of Solids (One or two weights) This is a rare experiment where you will get points for breaking a sample! The recommended textbooks and other
More informationExperiment Five (5) Principal of Stress and Strain
Experiment Five (5) Principal of Stress and Strain Introduction Objective: To determine principal stresses and strains in a beam made of aluminum and loaded as a cantilever, and compare them with theoretical
More informationSERVICEABILITY LIMIT STATE DESIGN
CHAPTER 11 SERVICEABILITY LIMIT STATE DESIGN Article 49. Cracking Limit State 49.1 General considerations In the case of verifications relating to Cracking Limit State, the effects of actions comprise
More informationA CRITERION OF TENSILE FAILURE FOR HYPERELASTIC MATERIALS AND ITS APPLICATION TO VISCOELASTICVISCOPLASTIC MATERIALS
MTS ADHESIVES PROGRAMME 19961999 PERFORMANCE OF ADHESIVE JOINTS Project: PAJ1; Failure Criteria and their Application to ViscoElastic/ViscoPlastic Materials Report 2 A CRITERION OF TENSILE FAILURE FOR
More informationTesting and Analysis
Testing and Analysis Testing Elastomers for Hyperelastic Material Models in Finite Element Analysis 2.6 2.4 2.2 2.0 1.8 1.6 1.4 Biaxial Extension Simple Tension Figure 1, A Typical Final Data Set for Input
More informationObjectives: After completion of this module, you should be able to:
Chapter 12 Objectives: After completion of this module, you should be able to: Demonstrate your understanding of elasticity, elastic limit, stress, strain, and ultimate strength. Write and apply formulas
More informationCOURSE TITLE : THEORY OF STRUCTURES I COURSE CODE : 3013 COURSE CATEGORY : B PERIODS/WEEK : 6 PERIODS/SEMESTER: 90 CREDITS : 6
COURSE TITLE : THEORY OF STRUCTURES I COURSE CODE : 0 COURSE CATEGORY : B PERIODS/WEEK : 6 PERIODS/SEMESTER: 90 CREDITS : 6 TIME SCHEDULE Module Topics Period Moment of forces Support reactions Centre
More informationUNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationPhysics 3 Summer 1989 Lab 7  Elasticity
Physics 3 Summer 1989 Lab 7  Elasticity Theory All materials deform to some extent when subjected to a stress (a force per unit area). Elastic materials have internal forces which restore the size and
More information: APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4021 COURSE CATEGORY : A PERIODS/ WEEK : 5 PERIODS/ SEMESTER : 75 CREDIT : 5 TIME SCHEDULE
COURSE TITLE : APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4021 COURSE CATEGORY : A PERIODS/ WEEK : 5 PERIODS/ SEMESTER : 75 CREDIT : 5 TIME SCHEDULE MODULE TOPIC PERIODS 1 Simple stresses
More informationDeformation of Polymers. Version 2.1. Boban Tanovic, MATTER David Dunning, University of North London
Deformation of Polymers Version 2.1 Boban Tanovic, MATTER David Dunning, University of North London Assumed Preknowledge It is assumed that the user is familiar with the terms elasticity, stress, strain,
More informationDESIGN AND APPLICATION
III. 3.1 INTRODUCTION. From the foregoing sections on contact theory and material properties we can make a list of what properties an ideal contact material would possess. (1) High electrical conductivity
More informationSTRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS
1 UNIT I STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define: Stress When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The
More information1.105 Solid Mechanics Laboratory Fall 2003 Experiment 3 The Tension Test
1.105 Solid Mechanics Laboratory Fall 2003 Experiment 3 The Tension Test Our objective is to measure the Elastic Modulus of steel. The experiment comes in two parts. In the first, you will subject a steel
More informationStrength of Materials (15CV 32)
Strength of Materials (15CV 32) Module 1 : Simple Stresses and Strains Dr. H. Ananthan, Professor, VVIET,MYSURU 8/21/2017 Introduction, Definition and concept and of stress and strain. Hooke s law, StressStrain
More informationSupplemental Material for Monolithic Multilayer Microfluidics via Sacrificial Molding of 3D Printed Isomalt. M. K. Gelber and R.
Electronic Supplementary Material (ESI) for Lab on a Chip. This journal is The Royal Society of Chemistry 2015 Supplemental Material for Monolithic Multilayer Microfluidics via Sacrificial Molding of 3D
More information13 Solid materials Exam practice questions
Pages 206209 Exam practice questions 1 a) The toughest material has the largest area beneath the curve the answer is C. b) The strongest material has the greatest breaking stress the answer is B. c) A
More informationLecture 8 Viscoelasticity and Deformation
HW#5 Due 2/13 (Friday) Lab #1 Due 2/18 (Next Wednesday) For Friday Read: pg 130 168 (rest of Chpt. 4) 1 Poisson s Ratio, μ (pg. 115) Ratio of the strain in the direction perpendicular to the applied force
More informationCHAPTER 6: ULTIMATE LIMIT STATE
CHAPTER 6: ULTIMATE LIMIT STATE 6.1 GENERAL It shall be in accordance with JSCE Standard Specification (Design), 6.1. The collapse mechanism in statically indeterminate structures shall not be considered.
More informationTask 1  Material Testing of Bionax Pipe and Joints
Task 1  Material Testing of Bionax Pipe and Joints Submitted to: Jeff Phillips Western Regional Engineer IPEX Management, Inc. 20460 Duncan Way Langley, BC, Canada V3A 7A3 Ph: 6045348631 Fax: 6045347616
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationHardened Concrete. Lecture No. 16
Hardened Concrete Lecture No. 16 Fatigue strength of concrete Modulus of elasticity, Creep Shrinkage of concrete StressStrain Plot of Concrete At stress below 30% of ultimate strength, the transition
More informationStructural Metals Lab 1.2. Torsion Testing of Structural Metals. Standards ASTM E143: Shear Modulus at Room Temperature
Torsion Testing of Structural Metals Standards ASTM E143: Shear Modulus at Room Temperature Purpose To determine the shear modulus of structural metals Equipment TiniusOlsen LoTorq Torsion Machine (figure
More informationPharmaceutical compounding I Colloidal and SurfaceChemical Aspects of Dosage Forms Dr. rer. nat. Rebaz H. Ali
University of Sulaimani School of Pharmacy Dept. of Pharmaceutics Pharmaceutical Compounding Pharmaceutical compounding I Colloidal and SurfaceChemical Aspects of Dosage Forms Dr. rer. nat. Rebaz H. Ali
More informationLecture 15 Strain and stress in beams
Spring, 2019 ME 323 Mechanics of Materials Lecture 15 Strain and stress in beams Reading assignment: 6.1 6.2 News: Instructor: Prof. Marcial Gonzalez Last modified: 1/6/19 9:42:38 PM Beam theory (@ ME
More informationD : SOLID MECHANICS. Q. 1 Q. 9 carry one mark each. Q.1 Find the force (in kn) in the member BH of the truss shown.
D : SOLID MECHANICS Q. 1 Q. 9 carry one mark each. Q.1 Find the force (in kn) in the member BH of the truss shown. Q.2 Consider the forces of magnitude F acting on the sides of the regular hexagon having
More informationPES Institute of Technology
PES Institute of Technology Bangalore south campus, Bangalore5460100 Department of Mechanical Engineering Faculty name : Madhu M Date: 29/06/2012 SEM : 3 rd A SEC Subject : MECHANICS OF MATERIALS Subject
More informationEquilibrium. the linear momentum,, of the center of mass is constant
Equilibrium is the state of an object where: Equilibrium the linear momentum,, of the center of mass is constant Feb. 19, 2018 the angular momentum,, about the its center of mass, or any other point, is
More informationStresses in Curved Beam
Stresses in Curved Beam Consider a curved beam subjected to bending moment M b as shown in the figure. The distribution of stress in curved flexural member is determined by using the following assumptions:
More information